# Unusual Dynamic Processes in Polymer Nanocomposites · PDF file Unusual Dynamic Processes in...

date post

08-Jul-2020Category

## Documents

view

0download

0

Embed Size (px)

### Transcript of Unusual Dynamic Processes in Polymer Nanocomposites · PDF file Unusual Dynamic Processes in...

Unusual Dynamic Processes in Polymer Nanocomposites

Nigel Clarke Department of Physics and

Astronomy University of Sheffield, UK

5

0 5 10 15 20 25 30 35 40 φ %

0

0.2

0.4

0.6

0.8

1

1.2

1.4

1.6

D /D

0

Maxwell simulation, N=100 experiments, PMMA, NP50 experiments, PMMA, NP29 experiments, PMMA, NP13

R=1

FIG. 3. Dependence of diffusivity (normalized to its bulk value) of weakly-entangled polymers (N = 100) for different nanoparticle loading:(i) Maxwell prediction (black line) (ii) simulation data N = 100 (stars), (iii) PMMA tracer diffusion: diameter dNP = 13 nm (circles), (iv) dNP = 29 nm (squares), (v) dNP = 50 nm (triangles).

2. Weakly entangled polymers diffusion

We show in Figure 3 the diffusivity (as calculated from Eq. 2) of weakly entangled polymers (N = 100) as a function of the nanoparticle loading. We observe that the poly- mer diffusion decreases with the addition of nanoparticles in the matrix. We can see that the simulation data agree with the experimental system of PMMA tracer diffusion23, at high nanoparticle loadings. However, in the dilute noparticle regime there is discrepancy to the data. In the experimental nanocomposite, tracer diffusion23 collapses onto a mas- ter curve when the neat homopolymer diffusion (D/D0) is plotted versus a confinement parameter defined as the interparticle distance relative to the polymer radius of gyration (ID/2Rg)22,23,72 where the interparticle distance ID is given as: ID = 2R[(

2 πφ)

1/3 − 1], where, φ is the volume fraction of nanoparticles. However in our data, the mechanism of reduction of diffusion in our simulation data, is not due to entropic barriers but due to nanoparticle interfacial area73,74 and the act of nanoparticles as topological constraints75 in the matrix. In a simplified model where polymer chains were modeled as spheres diffusing down cylindrical pores76, it was shown that excluded volume effects can account for the observed reduction in polymer diffusion for values of ID/2Rg > 5. In that region, the ex- cluded volume model predicted a pseudomaster curve for the reduced diffusion coefficients, in good agreement with experimental results22,72 at higher nanoparticle loading. In addi- tion, in nanocomposites of poly(ethylene glycol) (PEG)-tethered silica (SiO2) nanoparticles and poly(methyl methacrylate) (PMMA), polymer chain dynamics undergoes a continuous transition from bulklike behavior at low nanoparticle loading to confinement behavior at intermediate nanoparticle loading and ultimately to glassy behavior at high nanoparticle loading77.

Acknowledgements

University of Sheffield • Argyrios Karatrantos

– Molecular dynamic simulations • Mike Weir

– Graphene oxide nanocomposites

University of Minho, Portugal • José Covas, Gabriel Bernando

– Structure/processing in C60 nanocomposites

DuPont Central R&D • Jeff Meth and Steve Zane

– Materials and characterisation

University of Pennsylvania • Karen Winey, Russell Composto • Minfang Mu, Wei-Shao Tung,

Mike Hore – Carbon nanotube

nanocompsites • Sangah Gam, Chia-Chun Lin,

Philip Griffin – Silica nanocomposites

Funding: NSF/EPSRC Materials World Network

Dynamics are important for polymer processing …

• Dispersion/orientation of nanoparticles during processing depends on dynamics of polymers and nanoparticles

• Dynamics characterised by the viscosity and the diffusion coefficient

By using this ability to transform NPs from hard to soft by reducing the matrix molecular weight, we have uncovered a universal scaling rule for polymer diffusion in nanocomposites. We previously found that PNCs with hard NPs (d ∼ 13 and 29 nm) capped with a phenyl group showed a monotonic slowing down of polymer dynamics with increasing confinement across a wide range of SiO2 NP concentration (ϕsilica = 0−0.5) and tracer molecular weight (Mn

t = 49−532 kg mol−1).23,24 In this paper, we investigate and compare diffusion in polymer nanocomposites containing hard and soft NPs and find that a simple confinement parameter can capture the correlation between dynamics and structure. Surprisingly, by defining an effective particle diameter that accounts for tracer penetration into the brush in soft NP systems, polymer diffusion is found to be universal for both hard and soft NPs over a wide NP concentration and tracer molecular weight. This universal scaling behavior highlights the importance of interparticle distance between hard/soft NPs relative to the size of the diffusing chain. To determine tracer diffusion coefficients, the volume

fraction profiles of deuterated polystyrenes (dPS) in PNCs are measured by elastic recoil detection (ERD).25 Bilayer samples were prepared with a top dPS (Mn

t = 23−1866 kg mol−1) layer of 15 nm on a thick polystyrene (PS; Mn

m = 160 kg mol−1, PDI = 1.05) nanocomposite containing either hard or soft nanoparticles (ϕsilica = 0−0.5). Bilayers were annealed in a vacuum oven at T = 170 °C for a few minutes to hours. Hard NPs were prepared by modifying SiO2 NPs (51 nm diameter, 0.22 dispersity) with low molecular weight initiator (2-bromo- isobutylate derivative) and are denoted as SiO2−I. Using the same SiO2 NPs, soft NPs are functionalized with polystyrene

brushes (Mn b = 87 kg mol−1 and ρ = 0.52 chains/nm2) grown

by surface-initiated atom transfer radical polymerization (SI- ATRP) and denoted as SiO2−PS87k.26−28 The inset of Figure 1 depicts the brush-grafted (red) NP with diameter d and brush thickness h in a PS matrix (black). To understand how tracer diffusion depends on the unoccupied volume in the PNC, the interparticle distance (ID) was precisely controlled by tuning the volume fraction of SiO2−PS87k or SiO2−I, while maintaining a uniform dispersion of NPs. The cross-sectional transmission electron micrograph in Figure 1 shows that nanoparticles are well dispersed in a PS matrix at ϕsilica ∼ 0.06. The surface modification of the NPs using polymer brushes and low molecular ligands facilitates the uniform dispersion in PS even up to extremely high loading, ϕsilica = 0.5. For the annealed bilayer (Figure 2a, inset), a representative

dPS volume fraction profile is shown in Figure 2a, where the solid line represents the best fit to the experimental data (circles). Using Fick’s second law and appropriate boundary and initial conditions, ϕdPS(x) is given by

ϕ = − + + ⎡ ⎣⎢

⎛ ⎝⎜

⎞ ⎠⎟

⎛ ⎝⎜

⎞ ⎠⎟ ⎤ ⎦⎥x

l x Dt

l x Dt

( ) 1 2

erf 4

erf 4dPS (1)

where erf, t, and l are the error function, annealing time, and initial dPS thickness, respectively. Equation 1 is convoluted with the instrumental depth resolution and chi squared fitting is used to determine the best fit (solid line), which corresponds to D = 1.8 × 10−14 cm2 s−1 in Figure 2a.29,30 Figure 2b shows the tracer diffusion coefficients for five tracer molecular weights (Mn

t = 23−1866 kg mol−1) as a function of the volume fraction of silica (ϕsilica = 0 to ∼0.06). At fixed ϕsilica, the diffusion

Figure 1. Morphology of SiO2−PS87k:PS nanocomposites. Cross-sectional TEM micrograph depicting the distribution of silica cores (d = 51 nm) for a nanocomposite film with ϕsilica ∼ 0.06. Inset shows the scheme of a polystyrene-grafted silica nanoparticle (Mnb = 87 kg mol−1, red) dispersed in a polystyrene matrix (Mn

m = 160 kg mol−1, black).

ACS Macro Letters Letter

dx.doi.org/10.1021/mz400064w | ACS Macro Lett. 2013, 2, 485−490486

78 Two phenyl-capped nanorods with similar aspect ratios (AR 79 ∼ 9) but different sizes, NR-short (TiO2; L = 43.1 nm and d = 80 4.6 nm) and NR-long (SiO2-[Ni(N2H4)3]Cl2; L = 371 nm and 81 d = 43 nm) were prepared using standard Schlenk-line 82 techniques.16,17 For NR-short and NR-long, the surfaces are 83 grafted with (chloromethyl)dimethyl phenylsilane that facilitate 84 uniform dispersion of NRs in a polystyrene (PS; Mn = 650 kg/ 85 mol) matrix, as shown in the cross-sectional transmission

f1 86 electron micrographs (Figure 1a,b), respectively. These NRs 87 are athermal in a PS matrix. To age the matrix, the film was 88 preannealed at 150 °C for 3 days. No change in NR dispersion 89 was observed, consistent with stable grafting. The glass 90 transition temperatures (Tg) of the nanocomposites were 101 91 ± 1 °C, consistent with the prior results for PS mixed with 92 phenyl-capped silica.6 For diffusion studies, bilayers with a top 93 deuterated polystyrene (dPS; Mn = 168−3400 kg mol−1) with a

94thickness of 15 nm are deposited on a thick PNC (ϕNR = 0− 950.1). Bilayers are annealed in a vacuum oven at T = 170 °C 96from a few hours to days. Tracer diffusion coefficients are 97determined by fitting the dPS volume fraction profiles 98determined by elastic recoil detection (ERD).7,18 A representa- 99tive dPS volume fraction (ϕdPS) profile is shown in Figure 1d, 100along with the best fit (solid line). 101The tracer diffusion coefficients of entangled polymers (Mn = 102168−3400 kg mol−1) in PNCs containing NR-short and NR- 103long are shown in Supporting Information, Figures S1 and S2 104 f2as a function of NR volume fraction, ϕNR. Figure 2 shows dPS 105tracer diffusion coefficients in PNCs with NR-long normalized 106by that in pure polymer melts versus ϕNR. For the smallest 107tracers (168 and 532 kg mol−1), normalized diffusion 108monotonically decreases as ϕNR increases, resulting in a nearly 10950% r